Agnieszka Bondyra, Pawe Gotowicki


 Osborne Harris
 1 years ago
 Views:
Transcription
1 Journal of KONES Powertrain and Transport, Vol. 17, No INFLUENCE OF A CROSSHEAD RATE AND A NUMBER OF STRESS CYCLES ON MEASUREMENT RESULTS IN THE INPLANE SHEAR TEST FOR A CROSSPLY VINYLESTERCARBON LAMINATE Agnieszka Bondyra, Pawe Gotowicki Military University of Technology Department of Mechanics & Applied Computer Science Gen. Sylwestra Kaliskiego 2 Street, 98 Warsaw tel.: , fax: Abstract The paper presents some experimental studies on a regular crossply laminate of the [(/9) F ] 4S configuration. Each layer is VE 11M vinylester resin (the manufacturer: OrganikaSarzyna Chemical Plants, Sarzyna, Poland) reinforced with pla in weave carbon fabric of parameters: S tyle 43, Carbon 6K, substance 3 g/m 2, warp/weft 4/4 tex, 3.7/ 3.7 yarn/cm (the manufacturer: C. Cramer GmbH & Co. KG Division ECC). The orthotropic laminate was produced by ROMA private enterprise in Grabowiec, Poland, using the vacuum molding method and the technological parameters developed by ROMA taking into account the VE 11M material specification. The PNEN ISO 14129:1997 standard [1] and closely related standards [29] were taken into consideration in experimental studies on the static inplane shear response by a tensile test of a [(±4) F ] ns laminate. A program of the experiments was focused on testing a rate of a testing machine crosshead and a number of sta tic stress cycles. An influence of these factors on the inplane shear modulus was investigated. Based on the conducted investigations, the modified experimental procedure has been proposed for determination of the correct value of the inplane shear modulus and the inplane shear strength. Keywords: vinylestercarbon laminate, regular crossply laminate,, inplane shear test, experimental procedure 1. Introduction Shear tests for polymermatrix composite materials are the most difficult tests for determining mechanical properties, particularly in the plane perpendicular to the laminate plane. There are wellknown numerous methods for shear tests of laminates. The most important of them are described below [113]. Two or three rails, which the specimens are attached to, are applied in the method of shear test in rails (ASTM D42/D42M1 [2]). This method defines the inplane shear modulus and the inplane shear strength. The length/width ratio for the measured region of the specimen is recommended to be greater than 1. The Iosipescu test method (ASTM D379/D379M [3]) uses fourpoint bending of the notched prismatic specimen. It allows determining the mechanical properties in all planes. Both methods require special instrumentation. The next method of a shear test applies a tensile test of a [(±4) F ] ns laminate (ISO 14129:2 [1] or its American equivalent ASTM D318/D318M94 [4]). This method allows determining the shear stress,, and the shear strain,, for polymermatrix composites with large failure deformations. It can be also used to determine the value of the inplane shear modulus, G 12, reliable since it is based on the straight section of the initial  relation. The plate torsion test (PNEN ISO 131:27 []) allows only determining the inplane shear modulus (G 12 ). The test uses simultaneous loading of the plate supported at two corners along its diagonal with cones placed at corners along the other diagonal.
2 A. Bondyra, P. Gotowicki Another method is a torsion test of a rod with circular or rectangular crosssection (PNC8976 [6]), with or without a hole. The method, for determining the apparent interlaminar shear strength of fiberreinforced composites using a short beam (PNEN ISO 1413:21 [7]), is applied to laminates with thermoset or thermoplastic matrix, under condition of damage caused by the interlaminar shear. This method can be applied to classify or to control the quality the materials. Standards related to the interlaminar shear strength of the plastics, developed separately for aviation and cosmonautics, are as follows: PNEN 2377:1994 [8] for glass fiberreinforced composites, and PNEN 263:2 [9] for unidirectional carbon fiberreinforced composites. Besides the abovementioned methods, there exist the others, such as: the tube twisting method (this method gives the most reliable results), the shear test using the fourbar linkage (the inplane shear; this method gives correct results for the inplane shear strength, but it is not suitable for determining the shear modulus), shear of a specimen in biaxial load (applied for many materials), torsion of ring specimens (applied in investigation of a pipeshaped laminate), shear of a specimen with notches (however, resulting in a large error) [12]. Originally, many of these test methods were dedicated to materials different from composites reinforced with continuous fibers (metals, wood, polymers). Some of them are not even standardized. Compatibility of these methods related to accuracy of determining the shear modulus is noted, whereas determining of the shear strength is more problematical. The edge effects, connecting of materials, nonlinear behaviour of the matrix or the matrixfibers connection, stress distribution (imperfections), existing of the normal stresses, cause that the value of the shear strength determined by existing methods is disputable. Therefore, the value of shear strength in engineering applications should be checked for each structure. Some of the test methods were proposed to determine the relation in a plane of the layer for fiberreinforced composites, the other ones are confined to the plane perpendicular to the previous one and some in dependence of cut of the specimen allow researching both cases. Summing up, the shear modulus and/or the shear strength are determined on the basis of the shear test. It is also possible to determine the failure strain. 2. Description of the experimental studies The aim of this study is to determine the influence of selected factors, i.e., a rate of the testing machine crosshead, a number of cycles of static stress, and sensors used for strain measurement, on the shear stress shear strain relation in the inplane shear test [1]. There is considered a vinylestercarbon regular crossply laminate denoted with the C/VE code. The modified procedure will be developed related to the test method presented in PNEN ISO standard [1]. It results from the fact that this standard does not take into account abovementioned factors Description of the test method The shear test method corresponds to the PNEN ISO standard [1] and permits to determine the shear stress,, and the shear strain,, of polymermatrix composites at large failure strain, without additional instrumentation. This method can be applied to determine the inplane shear modulus G 12. According to Ref. [1], the shear stress corresponding to % strain (if destruction of the specimen does not occur earlier) is assumed as a failure criterion. Such a criterion is also recommended by the ASTM D 318 standard [4]. According to Ref. [1], one load cycle is performed out at velocity given in a standard related to the tested material or 2 mm/min in case of lack of such data. Investigation was finished at =., if breaking of the specimen did not occur earlier. The shear modulus is defined in the interval of =.1., and the shear strength corresponds to the shear stress at the failure of the specimen or at =.. 3
3 Influence of a Crosshead Rate and a Number of Stress Cycles on Measurement Results in the InPlane Shear Test for... The method uses a tensile test of a [(±4) F ] ns laminate and can be applied in case of laminates with thermosetting matrices. The method is not suitable for investigation of laminates reinforced with thick fabrics. It is sensitive to number and distribution of the layers; the comparison is made using the same number of layers. The laminate of the ±4 symmetrical configuration can be made of unidirectional or fabrics reinforced layers, provided that the number of fibers in the warp and the weft is equal to each other. During the tests, the specimen in the form of a rectangular beam with the fibers oriented at the angle of ±4 to the specimen axis is subjected to an axial tension load. The fibers should be arranged symmetrically and in a sustainable manner with respect to the specimen axis. It should be noted that the specimen material during the measurement is not in a state of pure shear, since in the ±4 system there occur both shear and normal stresses. Uptodate studies show that the normal stresses exhibit only negligible influence on the value of the shear modulus, G 12, and only slightly decrease the shear strength, R 12 [12] The tested material The tests were carried out for the C/VE regular crossply laminate of [(/9) F ] 4S configuration. The Style 43 fabric was produced by the ECC using carbon fibers TenaxE HTA4, with fiber parameters provided in Tab. 1. The fabric is characterized by the following parameters: Style 43, a plain weave,.42 mm thickness, 1 mm width, 3 g/m 2 substance, 4/4 warp/weft, 3.7/3.7 yarn/cm. The vinylester resin VE 11M applied for laminates with increased requirements for chemical resistance and incombustibility was used to manufacture the considered composite. The VE 11M resin parameters are given in Tab. 2. Prefabricated laminate plates used in the investigations were produced by ROMA private enterprise; they were made using the vacuum molding method and the technological parameters developed by ROMA taking into account the VE 11M datasheet. Tab. 1. Properties of the fiber (manufacturer data) L.P. Property Unit Value 1 Sizing  E13 (Epoxy) 2 The content of the roving preparation % Number of filaments  6K (6) 4 Nominal linear density tex 4 Filament diameter m 7 6 Density g/cm Tensile strength MPa 39 8 Young s modulus at tension GPa Elongation at break .17 Tab. 2. Properties of the resin matrix (manufacturer data) L.P. Property Unit Value Standard 1 Tensile strength MPa 8 ISO Young s modulus at tension GPa 3. ISO Elongation at break % 3. ISO Flexural strength MPa 12 ISO 178 Young s modulus at bending GPa 4 ISO Temperature of deflection under load C 8 ISO Barcol hardness B 4 ASTMD
4 A. Bondyra, P. Gotowicki 2.3. Preparation of specimens Plates of mm dimensions, made using the vacuum molding method, were cut into small [(±4) F ] ns plates of length equal to the test specimen and of width appropriate for preparation of the required number of specimens. Additional cover plates were prepared in a similar manner. The cover plates were glued to the plate using a thin layer of adhesive (E3 epoxy resin), according to [1]. The glued surfaces were degreased and sandpapered. The combined parts were tightened until the resin has been polymerized (12 h). Plates, together with the cover plates, constituted the initial material for cutting the specimens. Rectangular prism shaped specimens were cut using a sawing machine with a diamond disk. The mechanically machined surfaces and edges of final specimens were free of imperfections visible through a magnifying glass with a low magnification. Further processing was performed by milling. For roughing, made on the numerically controlled CNC BFN 7SERVO AUTO milling machine, the speed 1 rpm and feed rate 898 mm/min were used, and for the final treatment 1 rpm and 1224 mm/min, respectively. After the final treatment, the shape and dimensions of the specimens were compatible with standard [1] (Fig. 1, 2). Fig. 1. A shape and geometry of the specimen, according to Ref [1] Fig. 2. Specimens for the shear test According to Ref. [1], the formed shapes were conditioned for more than 88 hours at temperature of 23 ±1 C and relative humidity of ±1%. The tests were performed at the same conditions Instrumentation, measuring of the specimens, performing the tests A width of the specimens was measured using a calliper of.1 mm accuracy, a thickness measured of.1 mm accuracy using a micrometer with the 2 mm cylinder foot. The measurements 32
5 Influence of a Crosshead Rate and a Number of Stress Cycles on Measurement Results in the InPlane Shear Test for... were executed in accordance with Ref. [1]. Afterwards, the arithmetic mean of three measurement results was calculated. Longer edges of individual specimens were parallel with tolerance of.2 mm, therefore, respective standard requirements were fulfilled. The investigations were executed on the INSTRON 882 universal testing machine with hydraulic wedge grips (Fig. 3). Fig. 3. View of a specimen mounted in the hydraulic wedge grips Four different crosshead rates were used during the tests: 1, 2, and 1 mm/min. The circuit of the load measurement showed the total spreading load transferred by the specimen and it did not show the inertial deceleration at every applied crosshead rate. Using the FastTrack software, the measured values of displacement, force and deformation in real time were automatically recorded and saved on a hard disk with sampling frequencies of, 1, 2 and Hz, respectively. The measurement of deformation was performed in two directions, i.e., parallel and perpendicular to the axis of the specimen. Vishay strain gauges of the a6 mm measuring base, 12 resistance, sensitivity constant k = 2.8, and two extensometers axial, INSTRON , and transverse, INSTRON WE44E, were used, both of the 2 mm measuring base (Fig. 4). a) b) Fig. 4. A specimen with installed sensors: a) strain gauges b) extensometers 33
6 2.. Processing of the measurement results [1] A. Bondyra, P. Gotowicki The shear stress was calculated using the formulas resulting from rotation about the angle of 4 in uniaxial tension: F 12 ( F),,, (1) bh where: 12  the current inplane shear stress [MPa], F  the current load [N], b  width of the specimen [mm], h  thickness of the specimen [mm]. The inplane shear strength is equal to R ( Fm ), (2) where: F m  load at break of the specimen or load corresponding to the deformation 12 =., if the test was completed before the specimen s failure [N], R 12  the inplane shear strength (maximum shear stress before the moment of completion of the test or at the deformation 12 =.) [MPa]. The shear strain is determined from the formula resulting from the deformation in uniaxial tension and rotation about the angle of 4 in the layer plane, i.e., 12 x y, (3) where: 12  shear strain (total deformation related to the directions parallel and perpendicular to the axis of the specimen), x, y  normal strains in the directions parallel and perpendicular to the axis of the specimen ( x >, y <). The shear modulus is calculated from the initial quasilinear shear stress shear strain relation: 12'' 12' G, 12 (4) 12'' 12' where: G 12  shear modulus [GPa], 12  shear stress corresponding to the strain of 12 =.1, 12  shear stress corresponding to the strain of 12 =., The shear stress shear strain relation was determined for each specimen. 3. Test results and their analysis Evaluation of the usefulness of sensors used for strain measurements A comparative study was carried out in order to evaluate the usefulness of sensors for the strain measurement. Extensometers and strain gauges were installed on the same specimen (Fig. 4). Figure shows the results of the measurement using strain gauges and extensometers versus time, at the rate of crosshead v = 1 mm/min. Significant differences in the strain recorded by the axial and transverse strain gauges and similar values of the strain recorded by the axial and transverse extensometers can be observed. This is caused by the stress distribution in the specimen. Strain gauges measured the strain in a small area close to the axis of the specimen, whereas extensometers measured the strain of the region covering the entire width of the specimen (gauges base 6 mm, extensometers 34
7 Influence of a Crosshead Rate and a Number of Stress Cycles on Measurement Results in the InPlane Shear Test for... base 2 mm). The strain is the sum of the absolute values of strains x, y and the strain for both types of sensors, calculated in this way, will be similar. The disadvantage of strain gauges is found in a smaller range of measured strain and in lack of reusability. The advantage of extensometers is averaging of shear strains in a large area of the specimen, ease and simplicity of installation. The test (Fig. ) ends at time t 14 s which corresponds to strain value of =.. Values recorded by a transverse strain gauge at the moments of t 24 and 27 s, are caused by shortcircuiting. Taking into account the above preliminary analysis, only extensometers were used in further experiments.,3,3,2,2 [],1,1, Transverse strain gauge Axial strain gauge Transverse extensometer Axial extensometer t [s] Fig.. Strains versus time recorded by strain gauges and extensometers for the selected specimen 3.2. Results of the measurements and their analysis In order to determine influences of a rate of the testing machine crosshead and of a number of stress cycles on the static relationship , the loading program presented in Fig. 6 was assumed. Each specimen was subjected to five cycles of kinematic loading of a triangular shape, at intervals of 3' that protect finishing the reverse creep after each cycle. Each cycle contains a linear increase of the vertical displacement of the traverse up to. mm ( =..6) and a linear decrease to zero. Fig. 6. The loading program for testing selected factors in the shear test The kinematic loading was executed at constant speed v = 1, 2, or 1 mm/min of the traverse. In this way, four fivecycle  diagrams for subsequent specimens were obtained, as shown in Figs
8 A. Bondyra, P. Gotowicki 2 2 v=1 mm/min 1 [MPa] 1 cycle 1 cycle 2 cycle 3 cycle 4 cycle ,1,2,3,4,,6 Fig. 7. The  diagram for v = 1 mm/min (specimen No. 8) 2 2 v=2 mm/min 1 [MPa] 1 cycle 1 cycle 2 cycle 3 cycle 4 cycle ,1,2,3,4,,6 Fig. 8. The  diagram for v = 2 mm/min (specimen No. 9) 2 2 v = mm/min 1 [MPa] 1  cycle 1 cycle 2 cycle 3 cycle 4 cycle,1,2,3,4,,6 Fig. 9. The  diagram for v = mm/min (specimen No. 1) 36
9 Influence of a Crosshead Rate and a Number of Stress Cycles on Measurement Results in the InPlane Shear Test for v=1 mm/min [MPa] 1 1 cycle 1 cycle 2 cycle 3 cycle 4 cycle ,1,2,3,4,,6 Fig. 1. The  diagram for v = 1 mm/min (specimen No. 11) Analysis of the  hysteresis loops presented in Figs. 71 leads to the following conclusions: 1) The executed strain interval corresponds to a linear Hooke's law. Small curvatures of plots in each cycle and a hysteresis loop indicate the occurrence of viscoelastic strains nonnegligible for the tested crosshead rates and the stress range. Viscoelastic strains in the loading test are typical for laminates [14]. Evidence of this phenomenon is observed in the graph of the load versus time in the first cycle at v = 1 mm/min (specimen No. 8), shown in Fig. 11 and in the graph of the  diagram shown in Fig. 12 for the strain range of =.1. proposed by ISO [1] in order to determine the shear module. 2) Along with increase of the crosshead rate a width of the hysteresis loop decreases. It corresponds to decrease of rheological effects. 3) After the first load cycle the permanent strain of ~.2 value occurs. This strain corresponds to redistribution of the residual stresses in the laminate caused by the manufacture technology. During the stress increase in the first load cycle, there appear microcracks in the laminate, distributed quasiuniformly in the whole volume of the specimen. 4) In the second and subsequent load cycles, the permanent strain increase is negligible. Therefore, in the 2 nd, 3 rd, 4 th, th load cycles, further degradation of the laminate microstructure does not occur. ) In the interval =.1.2, the  relationship is quasilinear for the tested traverse velocities, and thus the viscoelastic strains in this interval can be neglected (Fig. 13). 3, 2, 2, [kn] load 1, 1, v=1 mm/min, cycle 1,, , time [s] Fig. 11. The axial tensioning force versus time for v = 1 mm/min in cycle 1 (specimen No. 8) 37
10 A. Bondyra, P. Gotowicki 2 2 [MPa] 1 1 v=1 mm/min, cycle 1,1,2,3,4, Fig. 12. The  diagram for v = 1 mm/min in a cycle 1oad its linear regression for =.1. (specimen 8) 2 2 [MPa] 1 1 v=1 mm/min, cycle 1,1,2,3,4, Fig. 13. The  diagram for v = 1 mm/min in a cycle 1oad its linear regression for =.1.2 (specimen 8) The values of the shear modulus, G 12, for subsequent cycles of kinematic loading and applied load rates, calculated on the basis of the quasilinear strain interval =.1.2, are presented in Tab. 3 and Fig. 14. Tab. 3. The shear modulus calculated for the strain interval =,1,2 Specimen No. v G 12 [GPa] [mm/min] cycle 1 cycle 2 cycle 3 cycle 4 cycle The values of the shear modulus, G 12, at the 2 nd, 3 rd and 4 th load cycles can be considered as independent of the velocity of the crosshead rate and of a number of the loading cycles. In the first cycle, the shear modulus is greater by 6.4% (an average value) when compared to the second cycle results. 38
11 Influence of a Crosshead Rate and a Number of Stress Cycles on Measurement Results in the InPlane Shear Test for... 4 G 12 [GPa] mm/min 2 mm/min mm/min 1 mm/min cycle Fig. 14. The dependence of the shear modulus on a number of the loading cycles and on the crosshead rate 4. Final conclusions Taking into account notation in the PNEN ISO standard [1] and detailed conclusions resulting from the experiments, the authors propose the following modified procedure concerning determination of selected mechanical properties of orthotropic laminates in the inplane shear test: 1) Execution of the initial loading cycle of the triangular shape (linear increase of the crosshead displacement up to. mm and a linear decrease to zero), at the crosshead rate of v = 2 mm/min) in order to redistribute the residual (technological) stresses in the specimen. 2) A 3 break after the initial loading cycle, in order to perform the reverse creep of the specimen. 3) Execution of the main test, i.e., linear increase of the crosshead displacement at the velocity of v = 2 mm/min until the break of the specimen appears or the limited strain =. is reached. Determination of the  diagram. 4) Determination of the shear modulus G 12 based on the =.1.2 interval, using the linear regression due to measurement fluctuations. ) Determination of the shear strength R 12 equal to the maximum value in the  diagram. Other requirements formulated in Ref. [1], related to the specimen s preparation and conditioning, the experiment performing and processing of the measurement results, are fully accepted and applied in this study. References [1] PNEN ISO 14129:2, Material composites reinforced with a fib re. Determination of th e shear stress and the respective strain, shear modulus and shear strength in the in plane shear test by a tensile test of a ±4 laminate [in Polish]. [2] ASTM D42/D42M1:27, Standard test method for inplane shear properties of polymer matrix composite materials by the Rail Shear Method. [3] ASTM D379/D379M:1998, Standard test method for shear properties of composite materials by the VNotched Beam Method. [4] ASTM D318/D318M94:27, Standard test method for inplane shear response of polymer matrix composite materials by tensile test of a ±4 laminate [] PNEN ISO 131:27, Material composites reinforced with a fib re. Determination of th e inplane shear modulus using the plate torsion method [in Polish]. [6] PNC8976:1974, Plastics, Determination of a temperature dependent shear modulus at torsion [in Polish]. 39
12 A. Bondyra, P. Gotowicki [7] PNEN ISO 1413:21, Material composites reinforced with a fib re. Determination of th e conventional interlaminar shear strength using the short beam method [in Polish]. [8] PNEN 2377:1994, Aeronautics and cosmonautics. Plastics rein forced with g lass fibres. A method for determination of conventional interlaminar shear strength [in Polish]. [9] PNEN 263:2, Aeronautics and cosmonautics. Plastics reinforced with carbon fibres. Unidirectional laminates. Determin ation of co nventional interlaminar shear strength [in Polish]. [1] Tarnopol skii, Y. M., Arnautov, A. K. and Kulakov, V. L.: Methods of determination of shear properties of textile composites. Composites Part A, Applied Science and Manufacturing Vol. 3, No. 7, pp , [11] Van Paepegem, W., De Baere, I., Degrieck, J., Modelling the nonlinear shear stress strain response of glass fibrereinforced composites, Part I, Experimental results, Composites Science and Technology, Vol. 66, No. 1, pp , 26. [12] Ochelski, S., Experimental methods in mechanics of structural composites [in Polish], WNT, 24. [13] Miracle, D. B., Donaldson, S. L., ASM Handbook, Vol. 21: Composites, ASM International, 21. [14] Klasztorny, M., Niezgoda, T., Viscoelastic modeling of regu lar crossply laminates, Kompozyty (Composites), Vol. 9, No. 3, pp , 28. Acknowledgements This work is a part of a project No. O R 62 6 funded in by Ministry of Science and Higher Education, Poland. This support is gratefully acknowledged. The work was supervised by Professor M. Klasztorny, PhD, DSc, Military University of Technology, Warsaw, Poland. 4
Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationPhysical Properties Testing Technical Bulletin
Technical Bulletin MANUFACTURER Raven Lining Systems 13105 E. 61 st Street, Suite A Broken Arrow, OK 74012 (918) 6150020 TENSILE TESTING OF PLASTICS ASTM D638, ISO 527 Tensile tests measure the force
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationInsitu local strain measurement in textile composites with embedded optical fibre sensors
Insitu local strain measurement in textile composites with embedded optical fibre sensors S. Daggumati, E. Voet, I. De Baere, W. Van Paepegem & J. Degrieck Ghent University, Department of Materials Science
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationStructural Metals Lab 1.2. Torsion Testing of Structural Metals. Standards ASTM E143: Shear Modulus at Room Temperature
Torsion Testing of Structural Metals Standards ASTM E143: Shear Modulus at Room Temperature Purpose To determine the shear modulus of structural metals Equipment TiniusOlsen LoTorq Torsion Machine (figure
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationReliable Test Results
Intelligent testing Johannes J.Bührle  Agenda Reliable test results are a fundamental and highly topical aspect of materials testing. Using suitable examples we would like to show you how we view this
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationBE Semester I ( ) Question Bank (MECHANICS OF SOLIDS)
BE Semester I ( ) Question Bank (MECHANICS OF SOLIDS) All questions carry equal marks(10 marks) Q.1 (a) Write the SI units of following quantities and also mention whether it is scalar or vector: (i)
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationA CRITERION OF TENSILE FAILURE FOR HYPERELASTIC MATERIALS AND ITS APPLICATION TO VISCOELASTICVISCOPLASTIC MATERIALS
MTS ADHESIVES PROGRAMME 19961999 PERFORMANCE OF ADHESIVE JOINTS Project: PAJ1; Failure Criteria and their Application to ViscoElastic/ViscoPlastic Materials Report 2 A CRITERION OF TENSILE FAILURE FOR
More informationThe Relationship between the Applied Torque and Stresses in PostTension Structures
ECNDT 6  Poster 218 The Relationship between the Applied Torque and Stresses in PostTension Structures Fui Kiew LIEW, Sinin HAMDAN * and Mohd. Shahril OSMAN, Faculty of Engineering, Universiti Malaysia
More informationNONDESTRUCTIVE EVALUATION METHODS FOR COMPOSITE PILES
NONDESTRUCTIVE EVALUATION METHODS FOR COMPOSITE PILES John F. Davila Graduate Research Assistant 2006 URIUPRM SUMMER INTERNSHIP RESEARCH PROGRAM Kingstown, RI July 29 of 2006 PRESENTATION OUTLINE Introduction
More informationExperimental Study and Numerical Simulation on Steel Plate Girders With Deep Section
6 th International Conference on Advances in Experimental Structural Engineering 11 th International Workshop on Advanced Smart Materials and Smart Structures Technology August 12, 2015, University of
More informationCIVL222 STRENGTH OF MATERIALS. Chapter 6. Torsion
CIVL222 STRENGTH OF MATERIALS Chapter 6 Torsion Definition Torque is a moment that tends to twist a member about its longitudinal axis. Slender members subjected to a twisting load are said to be in torsion.
More informationFIS Specifications for Flex Poles (Edition May 2008) Original Text: German
FIS Specifications for Flex Poles (Edition May 2008) Original Text: German 1 Field of Application and Basic Information The following FIS specifications for flex poles are intended to ensure that flex
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationEXPERIMENTAL AND NUMERICAL ANALYSIS OF A LAMINATED BASALT COMPOSITE PLATE SUBJECTED TO BLAST LOAD
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 EXPERIMENTAL AND NUMERICAL ANALYSIS OF A LAMINATED BASALT COMPOSITE PLATE SUBJECTED TO BLAST LOAD Süleyman Baştürk 1,
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationMarch 24, Chapter 4. Deflection and Stiffness. Dr. Mohammad Suliman Abuhaiba, PE
Chapter 4 Deflection and Stiffness 1 2 Chapter Outline Spring Rates Tension, Compression, and Torsion Deflection Due to Bending Beam Deflection Methods Beam Deflections by Superposition Strain Energy Castigliano
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationTINIUS OLSEN Testing Machine Co., Inc.
Interpretation of StressStrain Curves and Mechanical Properties of Materials Tinius Olsen has prepared this general introduction to the interpretation of stressstrain curves for the benefit of those
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationOnline Calculation of Guide Rings for Hydraulic Cylinders
Online Calculation of Guide Rings for Hydraulic Cylinders Fietz Roland Haraldsson Anna 1 Outline 1 2 3 4 5 6 7 Guide Rings General Information / Introduction Guide Rings Synthetic Materials Demarcation
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationISO 178 INTERNATIONAL STANDARD. Plastics Determination of flexural properties. Plastiques Détermination des propriétés en flexion
INTERNATIONAL STANDARD ISO 178 Fifth edition 20101215 Plastics Determination of flexural properties Plastiques Détermination des propriétés en flexion Reference number ISO 178:2010(E) ISO 2010 PDF disclaimer
More informationSPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION
AIAA225 SPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION Neil Wahl Montana Tech of The University of Montana Butte, Montana 597 Daniel Samborsky John Mandell Douglas
More informationDesign of reinforced concrete sections according to EN and EN
Design of reinforced concrete sections according to EN 199211 and EN 19922 Validation Examples Brno, 21.10.2010 IDEA RS s.r.o. South Moravian Innovation Centre, U Vodarny 2a, 616 00 BRNO tel.: +420511
More informationDIGITAL IMAGE CORRELATION TECHNIQUE IN MEASURING DEFORMATION AND FAILURE OF COMPOSITE AND ADHESIVE
DIGITAL IMAGE CORRELATION TECHNIQUE IN MEASURING DEFORMATION AND FAILURE OF COMPOSITE AND ADHESIVE Ab Ghani A. F Sustainable Maintenance Engineering Research Group, Universiti Teknikal Malaysia Melaka,
More informationPoisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics
10.1111/j.14602695.2007.01095.x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationLongterm behaviour of GRP pipes
Longterm behaviour of GRP pipes H. Faria ( 1 ), A.Vieira ( 1 ), J. Reis ( 1 ), A. T. Marques ( 2 ), R. M. Guedes ( 2 ), A. J. M. Ferreira ( 2 ) 1 INEGI  Instituto de Engenharia Mecânica e Gestão Industrial,
More informationDRAPING SIMULATION. Recent achievements and future trends. Dr. Sylvain Bel LGCIE University Lyon 1
DRAPING SIMULATION Recent achievements and future trends 1 Dr. Sylvain Bel LGCIE University Lyon 1 2 DRAPING SIMULATION Why? How? What? DRAPING SIMULATION WHY? Clamps Punch Fabric Die 1 2 Resin 3 4 Fig.
More informationDETERMINATION OF EI FOR PULTRUDED GFRP SHEET PILE PANELS. Abstract
DETERMINATION OF EI FOR PULTRUDED GFRP SHEET PILE PANELS Yixin Shao, Cynthia Giroux and Zeid Bdeir McGill University Montreal, Quebec, Canada Abstract The flexural rigidity, EI, plays an especially important
More informationDetermination of the Shear Buckling Load of a Large Polymer Composite ISection Using Strain and Displacement Sensors
Sensors 2012, 12, 1602416036; doi:10.3390/s121216024 Article OPEN ACCESS sensors ISSN 14248220 www.mdpi.com/journal/sensors Determination of the Shear Buckling Load of a Large Polymer Composite ISection
More informationImproved stress prediction in adhesive bonded optical components
Improved stress prediction in adhesive bonded optical components J. de Vreugd 1a, M.J.A. te Voert a, J.R. Nijenhuis a, J.A.C.M. Pijnenburg a, E. Tabak a a TNO optomechatronics, Stieltjesweg 1, 2628 CK,
More informationSIMPLIFIED METHOD FOR PREDICTING DEFORMATIONS OF RC FRAMES DURING FIRE EXPOSURE
SIMPLIFIED METHOD FOR PREDICTING DEFORMATIONS OF RC FRAMES DURING FIRE EXPOSURE M.A. Youssef a, S.F. ElFitiany a a Western University, Faculty of Engineering, London, Ontario, Canada Abstract Structural
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationOPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION
OPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION Luca Barbaresi, Federica Morandi, Juri Belcari, Andrea Zucchelli and Alice Speranza University
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationDECLARATION. Supervised by: Prof Stephen Mutuli
DECLARATION The work presented in this project is the original work, which to the best of our knowledge has never been produced and presented elsewhere for academic purposes... EYSIMGOBANAY K. J F18/1857/006
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More informationFailure interaction curves for combined loading involving torsion, bending, and axial loading
Failure interaction curves for combined loading involving torsion, bending, and axial loading W M Onsongo Many modern concrete structures such as elevated guideways are subjected to combined bending, torsion,
More informationStrainBased Design Model for FRPConfined Concrete Columns
SP230 57 StrainBased Design Model for FRPConfined Concrete Columns by N. Saenz and C.P. Pantelides Synopsis: A constitutive strainbased confinement model is developed herein for circular concrete columns
More informationImpact resistance of laterally confined fibre reinforced concrete plates
Materials and Structures/Matériaux et Constructions, Vol. 34, December 2001, pp 612618 SCIENTIFIC REPORTS Impact resistance of laterally confined fibre reinforced concrete plates P. Sukontasukkul 1, S.
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More information1. Demonstrate that the minimum cationtoanion radius ratio for a coordination number of 8 is
1. Demonstrate that the minimum cationtoanion radius ratio for a coordination number of 8 is 0.732. This problem asks us to show that the minimum cationtoanion radius ratio for a coordination number
More informationDEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS
DEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS THE INFLUENCE OF THE FORM OF A WOODEN BEAM ON ITS STIFFNESS AND STRENGTHI (REPRINT FROM NATIONAL ADVISORY COMMITTEE FOR AERONAUTICS REPORT
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationSpecial edition paper
Development of New Aseismatic Structure Using Escalators Kazunori Sasaki* Atsushi Hayashi* Hajime Yoshida** Toru Masuda* Aseismatic reinforcement work is often carried out in parallel with improvement
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationEXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES
EXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES D. Kakogiannis 1, D. Van Hemelrijck 1, J. Wastiels 1, S. Palanivelu 2, W. Van Paepegem 2, K. De Wolf 3, J.
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationExperimental Approach to Determine the Stress at a Section of Semi Circular Curved Beam Subjected to OutOfPlane Load Using Strain Rosette
Experimental Approach to Determine the Stress at a Section of Semi Circular Curved Beam Subjected to OutOfPlane Load Using Strain Rosette Rakshith N 1, Dr. D S Ramakrishna 2, Srinivasa K 3, Md Nadeem
More informationSHEAR CAPACITY OF REINFORCED CONCRETE COLUMNS RETROFITTED WITH VERY FLEXIBLE FIBER REINFORCED POLYMER WITH VERY LOW YOUNG S MODULUS
SHEAR CAPACITY OF REINFORCED CONCRETE COLUMNS RETROFITTED WITH VERY FLEXILE FIER REINFORCED POLYMER WITH VERY LOW YOUNG S MODULUS Hu Shaoqing Supervisor: Susumu KONO ** MEE8165 ASTRACT FRP with low Young
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationMechanics of Materials
Mechanics of Materials 2. Introduction Dr. Rami Zakaria References: 1. Engineering Mechanics: Statics, R.C. Hibbeler, 12 th ed, Pearson 2. Mechanics of Materials: R.C. Hibbeler, 9 th ed, Pearson 3. Mechanics
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationEffects of Basalt Fibres on Mechanical Properties of Concrete
Effects of Basalt Fibres on Mechanical Properties of Concrete A. M. ElGelani 1, C.M. High 2, S. H. Rizkalla 3 and E. A. Abdalla 4 1,4 University of Tripoli, Civil Engineering Department, Tripoli, Libya
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationMetrol. Meas. Syst., Vol. XVIII (2011), No. 2, pp METROLOGY AND MEASUREMENT SYSTEMS. Index , ISSN
Metrol. Meas. Syst., Vol. XVIII (2011), No. 2, pp. 323 334 METROLOGY AND MEASUREMENT SYSTEMS Index 330930, ISSN 08608229 www.metrology.pg.gda.pl INDUCTIVE SENSOR FOR WEIGHING OF MASS Janusz Lewandowski
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More information